SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez nos Conditions d’utilisation et notre Politique de confidentialité.
SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez notre Politique de confidentialité et nos Conditions d’utilisation pour en savoir plus.
The Thermal Performance of Hempcrete.The thermal performance of buildings is very complicated and this guide is not intended to be anauthoritative work on building physics. In order to explain the thermal performance of hempcrete it isuseful to start with the explanation of a few basic facts. Heat moves by three mechanisms, conduction,convection and radiation. However building regulations have generally focused on the heat lost byconduction and largely ignores the other two mechanisms. Consequently most building professionalshave become obsessed by the common measurement of conduction for materials, the U-value ofbuilding elements. The U-value gives a figure for the heat energy conducted through a square metre ofmaterial or building element for each degree difference in temperature on each side (in watts per squaremetre per degree centigrade).Unfortunately it is not normal practice in the UK to carry out post completion monitoring of thermalperformance. This raises several important questions:– If there is no checking, how do we know what works and what doesn’t? How can we hope to improve if we don’t know how good we are now? Can we ever hope to achieve zero-carbon buildings, when we are flying blind?To obtain the thermal conductivity of a material it is measured in a laboratory test using a hot plate/hotbox. The sample is monitored until a steady state heat flow is achieved. The nature of this test dries thematerial sample and therefore the actual performance of the material in real buildings, where a degreeof moisture is always going to be present, may be very different from the dry laboratory test.Consequently very few buildings perform thermally as predicted at the design stage. Some buildingsperform better, but it is widely understood that most fail to perform as well as anticipated by thedesigner.Figure 1: Hygrothermal response to relative humidity
Figure 2: Hygrothermal properties within pores of materialFigures 1 and 2 show the ways in which water can be present in hempcrete. A shows the totally drystate, which only occurs when there is no humidity present. B shows some water present in the pores ofthe material. This is the normal state that occurs up to about 90% Relative Humidity (RH). C showswater beginning to fill the pores of the hempcrete at very high levels of RH and D shows the state ofsaturation at 100% RH.Since buildings are known to be normally in the range of 40 to 70% RH, hempcrete is predominantly instate B. This small amount of moisture in the hempcrete plays an important role in its thermalperformance by adding a phase change property. This is where the change of water state from liquid tovapour, or back, stores or releases energy. The characteristic of water being able to be in liquid orvapour states at a wide range of temperatures is the cause of humidity in the air. Water is in vapourstate at the full range of normal building temperatures and it therefore has a direct bearing on thethermal performance of all building materials.There is no doubt that walls with the same U-values transmit heat at the same rate when they are in asteady state. However, walls in buildings are very rarely, if ever, in a steady state. In fact only aportion of the heat energy on one side of a wall is conducted through to the other side. The rest issimply stored and then released later. The higher the heat capacity of a material the greater its ability tostore heat. This dynamic performance is very important to buildings in most climates but particularly ina temperate climate.Heat capacity is normally expressed in J/kg, however since materials can vary significantly in density itis more useful to consider the thermal capacity of a cubic metre in order to appreciate how different
materials can perform. Figure 3 shows the heat capacity of different materials, including Tradical ®Hemcrete® wall mix.Figure 3:Thermal capacity of materialsOur weather gives temperatures that vary all the time but with an underlying 24 hour cycle (diurnalchanges). It stand to reason that materials and designs that can create a stable internal temperature,despite the external variations lead to buildings that require the minimum of heating or cooling.
Figure 4: Heat transfer following sudden coolingResearch by Prof. de Herd and Dr Arnaud Everard, using lab test figures input into WUFI software hasshown that 250mm thick Tradical® Hemcrete® walls subjected to (simulated) sudden cooling of 20oCtake 72 hours to reach a steady state of heat transfer (see figure 4) compared to 30 hours in cellularconcrete and 12 hours in mineral wool of the same thickness (see figure 5). The amount of energy lostfrom the internal environment in the first 24 hours is less in the Hemcrete® than mineral wool (despitethe mineral wool having better laboratory tested thermal conductivity performance) and less than halfthat of cellular concrete. This is represented by the red area on the graph).
Q24h [kJ/m2] → 229 → 146 → 187 → 410 ( Cement concrete → 3163 )Figure 5: Energy loss responseThe energy lost from the Hemcrete® in the first 24 hours Q24 was 187 KJ/m2, this equates to an averageheat loss of 0.11W/m2.K despite the fact that the measured U-value for this thickness of Tradical®Hemcrete® is 0.29W/m2.K. This is one striking example of how dynamic thermal performance can bevery different from predictions based on steady state figures.The thermal diffusivity is very low for hempcrete compared to many other materials, which means itwill take longer to change temperature (see figure 6).
Figure 6:Thermal diffusivityThis research also showed 250mm of Tradical® Hemcrete® could almost completely (98.5%) dampen asinusoidal change in external temperature of 20oC to 0oC over a 24hr cycle (see figure 7).Figure 7: Dampening of sinusoidal temperature change
Figure 8 shows the comparisons of the dampening factor of the hempcrete and other materials in thesame simulation. Mineral wool, which is generally considered as a very good insulation materialperforms worse than the hempcrete in this dynamic simulation despite the fact that 250mm is muchthicker than would normally be used. The table also shows the time shift. This is the time delay of thepeak temperature getting through the wall. The longer the time shift, the better because this defers thetime when the peak heat condition will occur within the building and if it is deferred beyond the 12hours then as the diurnal temperature change has occurred then the lower temperature means that thereis no heating continuing to increase the temperature and in fact there is cooling going on.Figure 8: Dampening factor of materialsFigure 9 shows the laboratory apparatus used by Prof. Arnaud at ENTPE to do the same tests in thelaboratory. These physical tests have given similar results as the WUFI simulations.
Figure 9:Laboratory testing suiteSignificant amounts of heat are lost from buildings through air leakage. This simply means the hot airleaks through gaps and takes the heat with it which dramatically reduces the overall thermalperformance of the building. Hempcrete is a monolithic material that is inherently airtight and it iseasy to build with to create buldings with high air tightness performance. The construction concept ofthe solid hempcrete walls is that there is no need for lots of complicated layers, just a simple solid castor sprayed wall. This high level of air-tightness minimises the heat lost through air leakage and drafts.Current building regulations require air leakage rates of below 10m3/h.m-2 at 50 pascals (Pa). Testscarried out on commercial Tradical® Hemcrete® buildings have achieved air leakage figures of around2m3/h.m-2 at 50 Pa. Extrapolation and predictions for new domestic hempcrete buildings predict figuresof around 1m3/h.m-2 at 50 Pa.It is beginning to be more widely understood how important it is to design and construct buildings thatperform in reality rather than just on paper. In order to do this we need to understand all the propertiesof materials and building elements and how these properties relate to the real performance. There is nodoubt that walls should prevent as much heat being lost as possible, and they should contribute to thefeeling of comfort within the building.
Figure 10: Thermal effusively of materialsThe thermal effusivity of hempcrete is low (see figure 10) which is why it feels warm to the touch. Thiswarm feeling greatly improves the thermal comfort of a building. Experience of hempcrete buildingsin France and of hemp and lime buildings at Haverhill, Suffolk shows that sub-conscious feelings ofthermal comfort (average between air temperature and wall temperature) are achieved at an airtemperature of 1 to 2 degrees lower than in conventional masonry structures. This means that you feelwarm even though the heating is turned down, saving hundreds of pounds per year in heating costs.The graphs of thermal capacity, diffusivity and effusivity (figures 3, 6 &10) show that the properties ofhempcrete are quite similar to wood. Hempcrete is normally used in combination with a timber frameand this similarity of thermal properties is useful when considering thermal bridging. It is important torecognize here that wood and timber frame construction using mineral wool or hydrocarbon basedinsulation materials has given wood a poor reputation in terms of its thermal performance. It is worthnoting that solid timber walling for example as log cabins are thermally very effective. It is only wherewood is being used as the frame for its excellent lightweight and adaptable structural performance thatit suffers this poor thermal reputation. Timber in a framed building is normally considered to be athermal bridge where it interrupts insulation and current building regulations require that repeating andnon-repeating thermal bridges are calculated and considered. They also set a limit on the non-repeatingthermal bridges. However timber framing used in combination with hempcrete does not behave as athermal bridge because of the similarity of good thermal performance in full thickness application.This gives hempcrete a significant advantage over other construction methods because it is free ofthermal bridges.
Figure 11: Climatic variations and internal conditions in the Lime Technology officeEven sophisticated computer simulations and laboratory tests can only go so far in the prediction ofthermal performance. The real test comes when real buildings are constructed and monitored. The newLime Technology office has 500mm thick Tradical® Hemcrete® walls and is currently being monitoredto check thermal performance. Figure 11 shows the mean external temperature (dotted red line) andmean RH (dotted blue line) during the month of April 2007, compared to the mean internaltemperatures (solid red line) and RH (solid blue line) over the same period. The graph clearlyillustrates that the Hemcrete® walls are creating a very stable internal environment, which is usually acharacteristic of heavyweight structures.
Figure 12: The Adnams Brewery projectFigure 13: The warehouseThe Adnams Brewery Distribution Centre (figures 12 and 13) passively regulates the internaltemperature of the warehouse using the combination of the good design and materials. It does not use
any mechanical hearting or cooling to maintain this stable temperature. The energy savings areconsiderable and ongoing thanks to the passive performance of the Hemcrete® and other naturalbuilding products used in the building in combination with good design and construction.Utilisations de mortierset bétons de chanvre (Maison Diocésaine Chalons en Champagne / 2004)Figure 14:Hemp-lime plaster for referblishmentHemp-lime plasters can also be used in the refurbishment of solid wall masonry structures to improvetheir thermal performance. Although they will not greatly improve the U-value of the wall, they willhave a beneficial effect on the buffering of humidity and temperature changes as well as improving theair-tightness through their method of application as a sealing coating and improve the feelings ofcomfort. In a recent French study 65mm of Tradical® hemp and lime plaster used as part of a range ofenergy saving measures reduced the heating bills of a traditional stone building by 75% (see figure 14).Hemcrete wall mix spray applied.Density 330kg/m3Thermal conductivity 0.07W/mKHeat capacity (est) 1400 J/kgK.Hemcrete wall mix shuttered and tamped.Density 330 to 480kg/m3Thermal conductivity 0.07 to 0.11W/mKHeat capacity 1400 to 1550 J/kgK.Hemp plasterDensity 700 to 950kg/m3